 Nano Express
 Open Access
 Published:
Enhanced Nonlinear Optical Effect in Hybrid Liquid Crystal Cells Based on Photonic Crystal
Nanoscale Research Letters volume 12, Article number: 449 (2017)
Abstract
Nonlinearoptical response of photorefractive hybrid liquid crystal (LC) cells has been studied by means of dynamic holographic technique in twowave mixing arrangement. The LC cells include nonuniform silicon substrates comprising a micrometerrange photonic crystal. A thin LC layer is set between silicon substrate and a flat glass substrate covered by a transparent (ITO) electrode. A dynamic diffraction grating was induced in the LC volume by the twowave mixing of laser beams with simultaneous application of DC electric field to the cell. Theoretical model of RamanNath selfdiffraction was developed. This model allows for calculation of nonlinear optical characteristics in thin samples on the base of twowave mixing experimental data, and with taking into account light losses on absorption and/or scattering. The hybrid LC cells demonstrate strong nonlinear optical effect, prospective for many applications in electrooptical microsystems, such as SLMs, as well as in multichannel systems.
Background
Among the main advantages of optical processing systems is their ability to utilize the high temporal and spatial bandwidth of photonics. A fundamental component in these systems is a device that modulates light. Spatial light modulators (SLM), imposing information onto optical data fields in optical information processing systems, for long have been considered essential for efficient exploitation of the speed, parallelprocessing, and interconnection capabilities inherent to optics. These devices generally modify the phase, polarization, amplitude, and/or intensity of a spatial light distribution as a function of electrical drive information or the intensity of another light distribution [1]. The advantages of liquid crystal electrooptic materials for SLM’s include their high birefringence and low voltage operation. Placing liquid crystals on top of silicon integrated circuitry was proposed in the early 1980’s to produce handheld displays [2]. Due to the widest manufacturing of silicon integrated circuits, which may contain photodetectors, amplifiers, and memory elements, the electrooptical liquid crystal on silicon (LCoS) SLM’s became a standard tool in the majority of optical laboratories. The next and highly desired step suggests the alloptical information handling, which could be achieved via lightcontrolled modification of the optical properties of the medium. Many of optically addressed SLM’s adopted the basic sandwich structure with the photoconductor transferring a bias voltage applied to the sandwich to a modulating material, e.g., liquid crystals in the liquid crystal light valve (LCLV) [3].
Almost all existing nonlinear optical effects have been observed in dyedoped LC compositions, in which the absorbing dye molecules trigger the LC director reorientation [4]. Alternatively, light action on the photosensitive molecules affects the order parameter of LC that, in turn, results in substantial and fast changes of the local refractive indices of the LC [5]. Last year, the popular photosensitive centers become nanoparticles embedded in the LC volume [6]. Not absorbing LC systems have also attracted a lot of interest as photorefractive purenematicLC light valves. The main nonlinear optical mechanism in LC is collective reorientation of molecules in a bulk of LC under laser excitation that often appears with applied electric field. In the present work, we use pure nematic LC. The nonlinear optical mechanism in such as LC cells suggests a surfaceinduced photorefractive effect, which changes the orientation of the LC molecules in the bulk initiated from the surface. This effect was investigated in LC cells containing different surface materials, such as photorefractive polymer layers [7, 8], conductive layers with embedded impurities [9], noble metal plates [10], and photorefractive crystals [11]. As a rule, the initial orientation of the molecules on a surface was the planar. Another kind of cells, which exhibit surfaceinduced photorefractive effect, consist of simple glass substrates covered with ITO electrodes and filled with a pure nematic LC, but the studied main feature is the homeotropic orientation of molecules [12, 13]. Such effect is studied in the present work. We use, however, hybrid cells where one of the substrates is a photonic crystal made from silicon. Enhancement of physical properties of materials deposited in nano or microstructured surfaces, including optical, electrical, and other properties becomes one of a priority direction of the fundamental nanoscience. In our research, we investigate the possibility of strengthening of nonlinear optical effect in an LC cell which is due to the influence of a microstructured surface of a substrate, which forms the cell.
To investigate the nonlinear optical properties in hybrid LC cells containing a reflective surface, we apply the dynamic holographic technique based on the twowave mixing of laser beams in the reflection geometry [14]. It is known that the dynamic holography is based on three main effects, which act simultaneously: (1) creation of periodic interference pattern inside a nonlinear medium with the help of two or more coherent laser beams; (2) modulation of the refractive index under action of this interference pattern; in our case, it means inducing a phase dynamic grating inside a nonlinear medium; (3) selfdiffraction of the recording beams on the dynamic grating. So far, the wavemixing is known as an effective technique for many applications in nonlinear optics (see, for example, [15]). Suffice it to mention spatial multiplexing and switching of laser beams, alloptical control of parameters of the beams, dynamic optical memory, logic, etc. In the present work, we demonstrate that this method can also be applied as a simple experimental technique to determine nonlinear optical characteristics of thin films. We have developed a mathematical approach to calculate the coefficient of nonlinear refraction in a Kerrlike medium, from which the nonlinear optical susceptibility can be determined. The mathematical model covers the selfdiffraction of waves in the RamanNath regime, i.e., for the condition of a thin grating. This approach generally is satisfied for the majority of thin samples that typically have thickness of up to tens of micrometers. Such media include also LC cells. Note that an alternative method to determine the optical nonlinear susceptibility of transparent materials is the zscan technique [16]. But we show that the twowave mixing method is rather simple for the experimental realization and is very suitable for the investigation of the dynamical media, including that that works only in the reflection geometry.
Methods
Materials and Samples
Structure of the hybrid LC cells is shown in Fig. 1. The hybrid cell has a sandwichlike type, is formed by glass and silicon substrates and filled with nematic LC; its edges are glued. The thickness of the nematic LC layer is 20 μm. The flat glass substrate is covered with ITO electrode. The second substrate is cut from a phosphorusdoped silicon wafer, its dimensions are 17 × 17mm^{2}. Its resistivity is 4.5 Ω⋅cm, its thickness is 380 μm, and its orientation is 〈100〉. The silicon substrate contains two areas, namely, a surface with periodic microstructured part, which is actually a photonic crystal in the micrometer range, and a flat part of the surface.
The three Si substrates, used in our investigation, are shown in Fig. 2. The microstructures represent etched pits arranged in a square matrix (the substrates 1 and 2) or in a triangular matrix (the substrate 3). The pits are square micropyramids, which differ by the shape, size, and arrangement. There are (1) regular pyramids, (2) truncated pyramids (pits), and (3) slightly truncated pyramids. Regular micropyramids are 2 μm in height, the same base’s side of 2 μm, and periodicity of 3 μm. Pits have similar parameters, but they are close packed. Slightly truncated pyramids have the base side 1.5 μm and periodicity 3.5 μm. The microstructures were formed on the polished side of the silicon wafer by standard photolithographic technique followed by anisotropic etching for the substrates 1 and 3, or by plasma etching for the substrate 2.
Two nematic LC were used: pure nematic 5CB (4×(npentyl)4cyanobiphenyl) and nematic mixture E7. In all cases, molecular orientation in a liquid crystal layer is homeotropic and it appears spontaneously at ITO and silicon surfaces with processing temperature being kept not higher then 50 °C. We have investigated four samples, which differ by the shape of microstructure and by the used LC. The samples with silicon substrates 1 and 2 consist of two parts: one part contains a miscrostructured surface, and the second part is a flat. In such samples we have the opportunity to compare the nonlinear response in a flat cell (containing a flat part of the Si substrate), and in a microstructured cell (containing a microstructured part of the Si substrate).
This way, in our experiments we have the following hybrid cells:

1)
abbreviated M1: glass substrate + ITO/5CB/Si substrate 1, microstructured surface

2)
abbreviated F1: glass substrate + ITO/5CB/Si substrate 1, flat surface

3)
abbreviated M2: glass substrate + ITO/5CB/Si substrate 2, microstructured surface

4)
abbreviated F2: glass substrate + ITO/5CB/Si substrate 2, flat surface

5)
abbreviated M3: glass substrate + ITO/5CB/Si substrate 3, microstructured surface

6)
abbreviated M4: glass substrate + ITO/E7/Si substrate 3, microstructured surface
Experimental Setup
Figure 3 shows the scheme of the experimental setup, which is based on the dynamic holographic method with twowave mixing. Continuous semiconductor Nd:YAG laser (frequency doubling, λ = 532 nm, P = 52 mW, singlemode generation) is a light source. By means of a beam splitter BS and a mirror M, the laser radiation is split into two beams B _{0} and B _{1}, converging on the cell at a small angle θ ≈ 0.01 rad. The input intensities I _{0} and I _{1} are equalized with the help of the filter F1, and in our case, I _{0} = I _{1} = 3.3 W/cm^{2}. A laser spot diameter on a cell is 1 mm.
Two laser beams B _{0} and B _{1} form an interference pattern inside the sample. Both incident beams have linear p polarization. So the intensity modulation interference pattern is created. The normal LC cell makes the angle δ with the bisector of B _{0} and B _{1}. The DC electric field is applied due to the source G with the voltage U controlled in the range from 0 to 15 V. The ITO glass substrate is set as the positive electrode. We measured intensities of the first diffraction orders {−1} and {2} by using photodiodes D1 and D2 via computercontrolled digital oscilloscope DO. The angles of cell rotation were adjusted to maximize the diffraction signal and appeared to be δ ≈ 40 − 55^{0} for different samples. These results coincide with the experiments of other groups (for example [9, 12]); the reason for such an effect is beyond the scope of our study.
Model of Selfdiffraction of Waves in RamanNath Approximation
Selfdiffraction of waves has been considered in several works [17, 18]. When the selfdiffraction of two input waves on the photoinduced thin refractiveindex grating takes place, many diffraction orders appear at the output. By measuring the intensities in the first diffraction orders, one can calculate the modulation depth of the grating (Δn). Since in the Kerrlike medium the condition Δn = n _{2} I _{0} is valid (where I _{0} is the intensity of the exciting beam), the coefficient of the nonlinear refraction n _{2} is possible to calculate.
In this section, we look for the solution for the diffraction efficiency of the first diffraction orders in the case of notshifted sinusoidal refractive index grating. Then intensities in symmetrical orders will be equal. The modeling is started from the wave equation, in which both the electric field \( \overrightarrow{E} \) and the modulated part of the dielectric permittivity Δε resulting from the Kerrlike nonlinear effect depend on the coordinate z (along the wave propagation):
where c is the light velocity in the vacuum, \( {\varepsilon}_0={n}_0^2 \) represents the dielectric permittivity of a medium and n _{0} is its refractive index. We will look for the solution of the wave equation (1) in the sum of all diffraction orders, which are plane waves polarized in the direction of the axis \( \overrightarrow{y} \):
where ω _{0} is the frequency of the laser radiation, \( \overrightarrow{r} \) is the coordinate, and “c. c.” denotes the complex conjugate term. In our representation, it is convenient to express the attenuation coefficient as α = α _{abs} + α _{sc}, which takes into account the losses of laser radiation both on absorption α _{abs} and scattering α _{ s }. Figure 4 shows the wavevector diagram of selfdiffraction in RamanNath approximation. It demonstrates that the wave of the mth diffraction order corresponds to the spatial direction described by the wavevector \( {\overrightarrow{k}}_m \). Diffraction orders m = 0 and m = 1 belong to two exciting beams B _{0} and B _{1}. The wavevector of the mth diffraction order is \( {\overrightarrow{k}}_m={\overrightarrow{k}}_0 m\overrightarrow{K} \), and \( \overrightarrow{K} \) is the wavevector of the photoinduced grating. The permittivity modulation Δε is defined in the form of a grating:
By substituting solution (2) and (3) into Eq. (1), one obtains the relation for a slow variable amplitude A _{ m } of the mth order:
where k _{ υ } = 2π/λ is the wavevector in the vacuum, and the mark “∗” denotes the complex conjugation. Since in our representation, the main recording beams of the orders m = 0 and m = 1 are identical at the input, as well as throughout the thickness of the sample, it follows that ε _{1} is a real and does not depend on the coordinate z (see [18]): \( {\varepsilon}_1(t)={\varepsilon}_1^{*}(t) \). For further transformation of Eq. (4), we introduce a new function \( {U}_m\left( z, t\right)={A}_m\left( z, t\right) \exp \left(\frac{1}{2}\alpha z\right) \exp \left( im\frac{\pi}{2}\right) \), designate T = exp(−αz) the losses of the light intensity in the medium, and define \( {\varepsilon}_1= T{\tilde{\varepsilon}}_1 \). By introducing a new variable \( \tilde{z}={k}_{\upsilon}/\left({n}_0 \cos \left(\theta /2\right)\right)\cdot \left(1 T\right)/\left(2\alpha \right) \), where θ is the converging angle, Eq. (4) may be written as:
where parameter ϕ is defined by \( \phi = T{\tilde{\varepsilon}}_1/\left(2{n}_0^2{ \sin}^2\left(\theta /2\right)\right) \).
In the conditions of the RamanNath approximation, it is possible to neglect the last term on the right part of the Eq. (5) (Ref. [18]), i.e., 2m(m − 1)/ϕ < < 1 for any m. Then by introducing a new variable \( \zeta =\tilde{z}{\tilde{\varepsilon}}_1(t) \), we obtain our main equation in the RamanNath approximation:
This relation formally is a wellknown representation for the Bessel function, so its solution may be expressed by means of Bessel functions in the form:
The Eq. (6) satisfies properties of symmetry \( {U}_0{U}_0^{*}={U}_1{U}_1^{*} \) for the pair of the main beams, as well as for all pairs of the diffracted beams (\( {U}_2{U}_2^{*}={U}_{1}{U}_{1}^{*} \)). Note that at z = 0, E _{0}(0, t) = E _{1}(0, t) ≠ 0, but E _{ m }(0, t) = 0 for m ≠ 0, 1, and then output intensities of the first diffraction orders I _{{−1}}(d, t) and I _{{2}}(d, t) will be equal and defined by a formula (see also [18]):
where d is the thickness of a nonlinear medium; I _{0} is the intensity of a laser beam; J _{1} and J _{2} are the Bessel functions of the first kind of the first and second orders, respectively. Since in our case, the intensities I _{0} and I _{1} are equal, i.e., 2I _{0} = I _{laser}, consequently, the value of ζ can be written as:
In a Kerrlike medium Δn = n _{2} I _{0}, where n _{2} represents the nonlinear refraction coefficient, then the final value of ζ has a more simple form:
The diffraction efficiency η of the first diffraction order is determined as η = I _{{−1}}/(TI _{0}). On the other hand, the diffraction efficiency may be obtained experimentally by measuring the intensity I _{{−1}} and the transmission coefficient of a cell T. The common formula (8) is valid to calculate the diffraction efficiency in a large range. For smaller diffraction efficiencies, η ≤ 2%, the good approximation will be only the first polynomial term of (8): η ≈ ζ ^{2}/4. Consequently, one can obtain a simple relation for n _{2}:
It should be noted that the derived Eq. (11) has the same form, as the equation which is conventionally obtained for the case of the diffraction of only one probe beam from a given refractive index grating (see, for example, Ref. [19]). But for large values of η, that is usual for LC cells, a more precise relations (8) and (10) should be used to calculate the values ζ and n _{2}.
Knowing the value n _{2}, one can define the nonlinear susceptibility of the medium with the help of the expression:
where ε _{ e } is the electric constant. In the case of nematic 5CB, we use the refractive index for the homeotropic orientation of molecules n _{0} = n _{⊥} = 1.51 as that of the ordinary refractive index; similarly for nematic mixture E7, n _{0} = n _{⊥} = 1.5268.
The developed theoretical approach is valid for thin films possessing Kerrlike optical nonlinearity, when the light losses on the both the absorption and scattering are large. Since the selfdiffraction method does not require an additional laser source as a probe, the twowave mixing becomes a simple method for diagnostics of optical nonlinearity of thin mediums including LC cells.
Results and Discussions
We suggest the nonlinear optical mechanism in hybrid LC cells to be a surfaceinduced photorefractive effect, which changes the orientation of the LC molecules in the bulk initiated from the surface [12, 13]. In the twowave mixing experiments, the sample is illuminated by a periodic light interference pattern formed by two coherent laser beams. This pattern creates a spatial charge modulation on the LCsubstrate interface. Resulting periodic distribution of the electric field on the surface stimulates modulation of the director orientation on the substrate. The reorientation of the molecules starts at the surface and spreads into LC volume.
Typical twowave mixing experimental performance with hybrid LC cells is shown in Fig. 5. In the absence of electric field, we observe a regular twodimensional structure of the main laser beams reflected from a microstructured substrate of the cell (Fig. 5a). After application of DC voltage, many diffraction orders appear aside every pair of the main beams due to excitation of refractive index grating inside the cell (Fig. 5b). In the case of flat cells F1 and F2, there is no multiscattering pattern, we observe only one center line after applying the voltage. We measured the intensities in the first diffraction orders {−1} and {+2} in the centre line in the steady state for all cells: flat cells and cells with microstructured surface. Then we calculated the diffraction efficiency according to η = Ī _{{−1}}/(TI _{0}), where Ī _{{−1}} is the average intensity of two first diffraction orders (Ī _{{−1}} = (I _{{−1}} + I _{{2}})/2) and T is the transmission coefficient of the cell.
Note, that the surfaceinduced photorefractive effect, exploited in our experiments, depends strongly on the rotation angle of the sample relative to the bisector of converge angle between two input waves (see e.g., [9, 12, 13]). Thus, with the normal position of the sample, when the plate of the sample is perpendicular to the waves’ bisector, no diffraction orders are observed. At the same time in our case, when the sample is rotated relative to this bisector, the photoinduced refractive index grating appears to be shifted relative to the light interference pattern. This effect should be manifested in the existing of energy transfer between diffraction orders. In the case of our hybrid cells and two laser beams with equal input intensities, we have observed that the difference of the intensities in the first diffraction orders does not exceed 10%. We have taken an average value between these two measured intensities that is used for further calculations of the coefficient of the nonlinear refraction. This value belongs to the accuracy range of our estimations of the nonlinear optical coefficients. Also note that the developed mathematical model is reduced to rather simple resulting formula and does not include the changes of wave phases in a volume of a nonlinear layer. The effect of nonlocal response in the medium and the energy transfer between waves will be considered carefully in our next works.
In Table 1, we gather experimental parameters measured for the hybrid LC cells. The transmission coefficient is defined as T = I ^{out}/I _{0}, where I _{0} is the intensity of a single incident beam, and I ^{out} is the intensity of the output beam. T includes two parts: T = R _{ s } T _{ a }, where R _{ s } takes into account the intensity loss for scattering from the microstructured surface to form a periodic light pattern; and T _{ a } = exp(−αd _{eff}) describes intensity loss on absorption during light propagation in a bulk of LC cell. In Table 1 also we present the values d _{eff}, which is an effective thickness for a propagating beam in a cell. Note, in our measurements we neglect the losses on light reflection from input glass boundary of a cell.
Measured diffraction efficiencies for all cells in dependence on applied voltage are shown in Fig. 6. One can see that the diffraction efficiency reaches its maximum for a certain voltage, which differs in various cells; this voltage is higher for microstructured cells in comparison with flat one (compare F1 and M1, F2 and M2); as well as this voltage is changed in dependence on a shape of the microstructure (compare M1, M2, M3, M4). We also emphasize that the diffraction efficiencies reach rather large values in LC cells (up to 9% for the cells M1 and F1). We use measured values of η to calculate nonlinear optical characteristics of investigated LC cells, namely, the coefficient of nonlinear refraction n _{2} and effective nonlinear susceptibility χ ^{(3)}, taking into account that the LC cells possess Kerrlike optical nonlinearity.
Coefficients of nonlinear refraction calculated from experimental measurements of the diffraction efficiencies are shown in Fig. 7 for all cells. In the case of cells M1 and F1 as well as M3 and M4, n _{2} is calculated from the main formulas (8) and (10) as the measured diffraction efficiencies η > 3.5%. We use the approximate formula (12) for the cells M2 and F2, as the obtained η < 2%. We obtain that the maximal coefficient of nonlinear refraction is higher in a cell with microstructured substrate as compared with flat cells (see Fig. 7a, b). Table 2 presents the values of nonlinear susceptibility calculated from the maximal values of n _{2} in Fig. 7. Nonlinear susceptibility appeared to be essentially enhanced (by 30–100%) in the cells with microstructured substrate with respect to the cells made of flat substrates. Reasons leading to increasing modulation depth of the dynamical grating in the cells contained microstructured substrates are the subject for further research. We suppose this effect to be connected with initial reorientation of molecules arising on microstructured surface.
Conclusions
We have investigated the nonlinear optical effect in novel hybrid LC cells based on a silicon photonic crystal. The cell consists of two different materials separated by a thin LC layer with homeotropic orientation of molecules. One material is a glass substrate with ITO electrode. The second one is silicon substrate with periodic microstructured surface. Microstructures in a shape of periodically arranged micropyramids are etched on the silicon surface by applying the chemical photolithography method or plasma etching one.
We apply the dynamic holography method with twowave mixing to define the efficiency of selfdiffraction of the dynamic grating induced in LC layer. A theoretical model for the RamanNath selfdiffraction, offered for calculating the diffraction efficiency in the first diffraction orders, have allowed us to determine the nonlinear refraction coefficient n _{2}, and nonlinear susceptilibity χ ^{(3)} of the cells. We have also made a comparative analyses of nonlinear parameters obtained for cells with and without microstructures. Nonlinear susceptibility appeared to be essentially enhanced (by 30 − 100%) in the microstructured cells with respect to the cells made of flat surfaces. The underlying mechanism of the optical nonlinearity is the surfaceinduced photorefractive effect in the pure nematic LC. The increased modulation depth of the refractive index might be connected with initial reorientation of the molecules arising on the microstructured substrate.
The developed theoretical approach could be valid for determination of nonlinear optical characteristics of thin films possessing Kerrlike optical nonlinearity, in which the losses on the both absorption and scattering are large, as well as in the either transmission or reflection geometries. Photorefractive hybrid LC cells are perspective as new samples of electrooptical microsystems, including multichannel SLMs. Additionally, twowave mixing technique in such nonlinear cells may be successfully implemented in multichannel couplers, switches, and optical communication lines. They may be also applied in networks, if to ensure the independent control of each channel in LCD structures.
Abbreviations
 5CB:

4′(npentyl)4cyanobiphenyl
 E7:

Liquid crystal mixture
 F1:

Hybrid LC cell, composed by flat part of Si plate 1/5CB/glass plate covered by ITO
 F2:

Hybrid LC cell, composed by flat part of Si plate 2/5CB/glass plate covered by ITO
 ITO:

Conductive layer of indiumtinoxide
 LC:

Liquid crystals
 M1:

Hybrid LC cell, composed by microstructured part of Si plate 1/5CB/glass plate covered by ITO
 M2:

Hybrid LC cell, composed by microstructured part of Si plate 2/5CB/glass plate covered by ITO
 M3:

Hybrid LC cell, composed by microstructured part of Si plate 3/5CB/glass plate covered by ITO
 M4:

Hybrid LC cell, composed by microstructured part of Si plate 4/E7/glass plate covered by ITO
 Si:

Silicon
References
 1.
Fisher AD, Lee JM (1986) The current status of two dimensional spatial light modulator technology. Proc Soc PhotoOpt Instrum Eng 634:352–371
 2.
Kaneko E (1987) Liquid crystal TV displays: principles and applications of liquid crystal display. KTK Scientific, Tokyo
 3.
Aubourg P, Huignard JP, Hareng M, Mullen RA (1982) Liquid crystal light valve using bulk monocrystalline Bi12SiO20 as the photoconductive material. Appl Optics 21(20):3706–3712
 4.
Khoo IC (2009) Nonlinear optics in liquid crystalline materials. Phys Rep 471:221–56
 5.
Iljin A (2011) Transient modulation of order parameter and optical nonlinearity in a chiral nematic liquid crystal. Mol Cryst Liq Cryst 543:143–7
 6.
Stamatoiu O, Mirzaei J, Feng X, Hegmann T (2011) Nanoparticles in liquid crystals and liquid crystalline nanoparticles. Top Curr Chem. 2011. doi:10.1007/128_2011_233.
 7.
Pagliusi P, Cipparone G (2002) Surfaceinduced photorefractivelike effect in pure liquid crystals. Appl Phys Lett 80(2):68–3
 8.
Kaczmarek M, Dyadyusha A, Slussarenko S, Khoo IC (2004) The role of surface charge field in twobeam coupling in liquid crystal cell with photoconducting polymer layers. Appl Phys 96:2616–2623
 9.
Parka J, Grudniewski T, Yu K, Dabrowski R (2004) Optically addressed holographic gratings in LC cells with different layers and high optical anisotropy liquid crystals. OptoElectronics Review 12(3):317–320
 10.
Abbott SB, Daly KR, D'Alessandro G, Kaczmarek M, Smith DC (2012) Hybrid liquid crystal protorefractive system for the photorefractive coupling of surface plasmon polaritons. J Opt Soc Am B 29(8):1947–1958
 11.
Bortolozzo U, Residori S, Huignard JP (2008) Beam coupling in photorefractive liquid crystal light valves. J Phys D Appl Phys 41:224007
 12.
Slussarenko SS (2001) Photorefractive effect in pure nematic liquid crystals. Europhys Lett 56(5):672–4
 13.
Zhang J, Ostroverkhov V, Singer KD, Reshetnyk V, Reznikov Y (2000) Electrically controlled surface diffraction gratings in nematic liquid crystals. Opt Lett 25(6):414–3
 14.
Klimusheva G, Bugaychuk S, Yu G, Kolesnyk O, Mirnaya T, Ishchenko A (2006) Fast dynamic holographic recording based on conductive ionic metalalkanoate liquid crystals and smectic glasses. Opt Lett 31(2):235–3
 15.
Hesselink L, Feinberg J, Roosen G. (Eds.) (2008) Cluster issue on controlling light with light. J. Phys. D: Appl. Phys. 41(22):220301224007.
 16.
SheikBahae M, Said AA, Wei T, Hagan DJ, Van Stryland EW (1990) Sensitive measurement of optical nonlinearities using a single beam. J Quant Electron 26:760–3
 17.
Chi M, Huignard JP, Petersen PM (2009) A general theory of twowave mixing in nonlinear media. J Opt Soc Am B 26(8):1578–7
 18.
Enns RH, Rangnekar SS (1974) Diffraction by a laser induced thermal phase grating. Canadian Journal of Physics 52(2):99–10
 19.
Yariv A, Yeh P (2003) Optical waves in crystals. New Jersey:Wiley and Son's, Inc, Hoboken
Acknowledgements
The authors greatly thank Ruslan Kravchuk from Institute of Physics in Kiev for the assistance in preparation of samples; as well as Sergey Slussarenko for the assistance in carrying out dynamic holographic experiments.
Funding
No payment is due on publication of this article. The article processing charge has been waived by BioMed Central.
Author information
Affiliations
Contributions
SB developed the dynamic holographic method for determination of nonlinear optical constants, created a holographic setup, developed the mathematical model to calculation of nonlinear optical characteristics from holographic experiments, carried out measurements of the holographic characteristics, and wrote the manuscript. AI took part in the preparation of the LC samples, took part in the development of the holographic setup, and drafted and corrected the manuscript. OL and LK provided the fabrication of the photonic crystals, prepared the microscopic photos of the Si substrates, and drafted the manuscript. LT carried out the measurements the diffraction efficiencies in the dynamic holographic experiments, calculated the optical constants of the samples, wrote and corrected the manuscript. All authors discussed the providing research, read and approved the final manuscript.
Corresponding author
Correspondence to Svitlana Bugaychuk.
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Publisher’s Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Cite this article
Bugaychuk, S., Iljin, A., Lytvynenko, O. et al. Enhanced Nonlinear Optical Effect in Hybrid Liquid Crystal Cells Based on Photonic Crystal. Nanoscale Res Lett 12, 449 (2017) doi:10.1186/s1167101722173
Received
Accepted
Published
DOI
Keywords
 Hybrid liquid crystal cell
 Photonic crystal
 RamanNath selfdiffraction
 Kerrlike nonlinear medium
 Nonlinear susceptibility
 Nonlinear refractive coefficient
PACS
 42.65.An
 81.07.Pr
 42.70.Df